T. K. Rout et al.
sumption of water having excess fluoride over a prolonged period leads to a chronic disease known as fluorosis
-. Fluoride is normally present in the form of fluoride ions in minerals, found in sedimentary (limestone
and sandstone) and igneous (granite) rocks, and leached out to contaminate water through geological processes.
Higher fluoride levels in the groundwater get through these minerals by volcanic and fumarolic processes. Dis-
solution of these barely soluble minerals depends on the water composition and the time of contact between the
source minerals and the water. Fluoride in drinking water may be beneficial or detrimental depending on its
concentration . The upper limit of fluoride concentration in the natural drinking water is 1.5 mg/L according
to the guidelines for drinking water quality -.
Natural water is becoming enriched with fluoride by the means of (a) geological processes, and (b) industry.
Water contamination by industry stems from many areas including: effluent discharge, fertilizers & pesticides,
fluorosilicone and fluorocarbon polymer synthesis, coke manufacturing, glass and ceramic manufacturing, elec-
tronics manufacturing, electroplating operations, steel and aluminum manufacturing, metal etching (with hydro-
fluoric acid), and wood preservatives. Average fluoride values for aluminium reduction plants are reported as
107 - 145 mg/L in waste water streams . Concentrations of an order of magnitude greater have been reported
for glass manufacturing, ranging from 1000 to 3000 mg/L of fluoride  . Fluoride wastes are also generated
in the steel manufacturing industry from the sintering and steel-making processes -. In the sintering plant
fluoride is found as an impurity of limestone, where both fluorspar (CaF2) and limestone are among the basic
materials used in steel making and as such, contributed as the principal source for this industry of fluoride con-
Incidences of high fluoride groundwater have been reported from 23 nations around the globe . Endemic
fluorosis has become a major geo-environmental health issue in many developing countries of the world. The
Bureau of Indian Standards outlined Indian standards stating that 1 mg/L was the maximum permissible limit of
fluoride with further remarks stating “the lesser the better” . Of the fluoride deposits of 85 million tons on
the earth’s crust, 12 million tons are found in India . Seventeen states in India are endemic for fluorosis 
. About 25 million people in India suffer from fluorosis and another 66 million are at risk . It was stated
in 1993 that crippling skeletal fluorosis might occur in people who have ingested fluoride of 10 - 20 mg per day
over 10 to 20 years. Early stages of skeletal fluorosis start with pain in bones and joints, muscle weakness, stiff-
ness of joints, and chronic fatigue. During later stages of fluorosis, calcification of the bones takes place; osteo-
porosis in long bones and symptoms of osteosclerosis appear where the bones become denser and develop ab-
normal crystalline structure . General skeletal fluorosis directly affects the economy of villagers (mostly
tribal populations) as it causes illness and debilitation not only in humans but also in their domestic animals, on
which they depend for their basic income . Asian countries mainly India and China are worst affected. In
1993, 5 million people in Mexico (about 6% of the population) were affected by fluoride in groundwater .
Fluorosis is prevalent in some parts of central and western China, caused not only by drinking fluoride that is in
the groundwater but also by breathing airborne fluoride released from the burning of fluoride-laden coal.
Worldwide such instances of industrial fluorosis are on the rise. Argentina in Latin America and East and North
Africa are also endemic. Dental fluorosis is also caused due to damage of tooth enamel by the fluoride ion.
Tooth enamel is made up of hydroxyapatite (87%) which is a crystalline calcium phosphate ; the hydroxide
ion of this enamel is displaced by the most stable fluorideion to form fluoroapatite, a trigger of dental fluorosis.
Humans are most prone to this during the first 7 years of life. Dental fluorosis has been characterized and re-
ported when fluoride ion intake levels rise above 1.5 mg/L for an extended period of time.
Several different materials have been used for defluoridation such as activated carbon (AC), tricalcium phos-
phate, synthetic ion exchangers, lime activated alumina, and alum. There have also been many methods devel-
oped to remove excessive fluoride from water including adsorption, ion exchange, precipitation, electrolysis,
donnan dialysis, and electro dialysis -. Among these methods, adsorption is still one of the most exten-
sively used and cheapest methods for defluoridation of water -. However, in recent years, a considerable
amount of attention from scientists has been devoted to the study of different types of low-cost materials for
fluoride uptake such as: spent bleaching earth, wollastonite and chine clay, bentonite and activated bentonite,
kaolinitic clay, agricultural by-products, fly ash, carbon slurry, biogas residual slurry, zeolite, bone char, and
flax shive -. Literature research has shown that alumina supported on carbon nanotubes (Al2O3/CNT)
has a saturation adsorption capacity of 39.4 mg/g fluoride uptake. It is also found that the adsorption capacity of
Al2O3/CNT is 3.0 - 4.5 times that of γ-Al2O3 while almost equal to that of IRA-410 polymeric resin at 25˚C. The
adsorption isotherms of fluoride on Al2O3/CNT fit the Freundlich equation well with the optimal pH ranging
T. K. Rout et al.
from 5.0 to 9.0. Crystalline and hydrous iron (III)-zirconium (IV) hybrid oxide (IZHO) at the optimum pH range
between 4.0 and 7.0 provides good efficiency of fluoride uptake  . The kinetic data obtained for fluoride
adsorption on IZHO at pH 6.8 (±0.1) and room temperature (303 ± 2 K) described that both the pseudo-first-
order and the reversible first-order equations are equally well (r2
= ~0.98 - 0.99), and better than the pseudo-
second-order equation (r2
= ~0.96 - 0.98) for higher concentrations (12.5 and 25.0 mg/dm3
) of fluoride uptake.
The synthesis of a zirconia/multi-walled carbon nanotube (ZrO2/MWCNTs) hybrid is also a novel sorbent for
water defluoridation. The ZrO2/MWCNTs were significantly more effective in fluoride removal than all other
sorbents tested before, including ZrO2 impregnated carbons. The kinetics of fluoride adsorption on the mixed
oxide is driven by boundary layer diffusion -.
Recently, many researchers have worked on cost-effective fluoride adsorbents such as zeolites, metal-polymer
& metal-metal oxide composites as well as biomass materials like fishbone charcoal, Cynodon dactylon, chito-
san, acacia Arabica plant, and Tamarindus indica. Mostly, biosorption adsorbents have shown the fluoride re-
moval to be no better than 88%, though this is still better than a metal oxide system. It has been proven that bio-
sorption has good affinity selectively for ion uptake from aqueous solutions -.
The present work focuses on a hybrid system for fluoride uptake where a low-cost biosorbent, using Bermuda
grass (i.e., Cynodon dactylon) that is specially processed, leads to a novel fibrous material that once obtained
and impregnated with titania and iron oxide in-situ by thermal chemical vapour deposition (thermal-CVD) tech-
nique, is ready for fluoride uptake.
2. Materials and Methods
2.1. Processing of Bermuda Grass
Bermuda grass is a natural bio fiber that is abundantly available in India which was specially processed for our
investigation. The cleaned dry grass was pulverized and the fibrous powdered material was washed well with
doubly distilled water to remove the free acid, followed by thermal treatment using chemical vapour deposition
(CVD) setup at a heating rate of 50˚C/min in the presence of flowing N2 (250 mL/min). The heating continued
up to a final temperature of 600˚C, where it was held for 5 minutes, to obtain thermally activated carbon without
using any catalysts. The resulting product was cooled to room temperature and sieved to the desired particle
sizes, namely 200 - 325 mesh (74 to 44 µm). Finally, the product was stored in vacuum desiccators until re-
quired for further experiments.
2.2. Conversion of Micro Carbon Fiber to Nano Carbon Fiber Using Nano-Oxides
The next set of experiments was conducted using catalysts such as TiO2 and Fe2O3 nano powders. Titania was
procured from Aldrich chemical supplier whereas nanoiron oxide is plentiful available in our mill as waste by
product of hot rolling steel. These catalysts were mixed with pulverized raw grass powder in the ratio of 1:100
(catalyst to grass powder) and fed into the CVD set up at a heating rate of 50˚C/min in the presence of N2 flow
(250 mL/min). The dwell time of the mixed samples was 1 h each and the rate of cooling was the same as that of
heating. We could ascertain the optimum temperature for obtaining Fe2O3 based carbon nanofiber and TiO2
based carbon nanofiber is 800˚C from their respective phase diagrams for carbide formation.
2.3. Fluoride Adsorption Study
In the present study, the derived nanocomposites were utilized for the removal of fluoride from its aqueous solu-
tion. The sorption isotherm and kinetics experiments were performed by batch adsorption experiments and were
carried out by mixing 0.5 g (obtained by the study of effect of adsorbent dose) of sorbent with 100 mL of water
containing sodium fluoride at 10 mg/L as initial fluoride concentration. The mixture was agitated in a thermo-
static shaker at a speed of 250 rpm at room temperature. The defluoridation studies were conducted for the op-
timization of various experimental conditions like contact time, initial fluoride concentration, adsorbent dose,
and fluoride uptake with fixed dosage by varying pH. All of the experiments were carried out at 30˚C ± 5˚C
temperature. Fluoride ion concentration was measured with an automatic ion analyzer using the equipment
model Metrohm-TitriC based on ion chromatography principle and the pH of the solution was also measured by
Orion ion selective equipment. All other water quality parameters were analyzed by using standard methods .
The effects of different dosages of biosorbent on fluoride uptake were studied by keeping the initial fluoride
T. K. Rout et al.
concentration and volume of the solution steady at 10 mg/L and 100 mL, respectively, at pH 4.
The fluoride concentration is retained in the adsorbent phase, qe (mg/g), was calculated according to ,
( )Co Ce
= ⋅ (1)
where qe is the amount of fluoride adsorbed (mg/g), Co and Ce are the original/initial and residual concentration
at equilibrium (mg/L), respectively, of fluoride in solution, w is the weight of bi-adsorbents and V is the volume
2.4. Theory of Isotherm Models
The abilities of two widely used isotherms such as the theoretical Langmuir and empirical Freundlich isotherms,
to model the adsorption equilibrium data were examined. These models allow for an explanation about the na-
ture of adsorption from the shape of the curve. Langmuir adsorption isotherm  is perhaps the best known of
all isotherms, which is often applied in solid/liquid systems to describe the saturated monolayer adsorption. The
linear form of the equation is used to describe the adsorption capacity for a particular range of adsorbate con-
centration. It can be represented as:
qm Ka qm
= + (2)
where Ce is the equilibrium concentration (mg/L), qe is the amount of ion adsorbed (mg/g), qm is a constant for
a complete monolayer (mg/g), and Ka is an adsorption equilibrium constant (L/mg). The constants qm and Ka
can be determined from a linearized form of Equation (2) by the slope of the linear plot of Ce/qe versus Ce.
The Freundlich adsorption isotherm  is based on adsorption on a heterogeneous surface and is the earliest
known relationship describing the adsorption equilibrium. The linear form of this equation is given by:
log log logFqe K Ce
= + (3)
where qe is the amount of ion adsorbed (mg/g), Ce is the equilibrium concentration (mg/L), KF and 1/n are em-
pirical constants indicating the adsorption capacity and adsorption intensity, respectively. The plot of log qe
versus logCe of Equation (3) results in a straight line and from the slope and intercept of the plot, the values
for n and KF can be obtained.
2.5. Instrumental Analysis
The surface morphology and size distribution of the micro carbon fiber and nanocomposites were analyzed by
means of scanning electron microscopy (SEM) and transmission electron microscopy (TEM). The crystallinity
and structure of the nanocomposites and the as-prepared activated carbon from grass were analyzed by X-ray
3. Results & Discussion
3.1. XRD, SEM, and TEM Analysis for Nanocomposites
The X-ray diffraction patterns have demonstrated that there were no peaks to indicate a crystalline structure
(Figure 1(a)) of thermally treated grass at 600˚C. The absence of diffraction peaks confirms this material con-
sists of amorphous fibers. XRD patterns of iron oxide and titania induced fiber showed a number of diffraction
peaks for each which confirma crystalline product. In the case of iron oxide, the XRD shows the presence of
magnetite, iron nitride and iron carbide (Figure 1(b)); while for titania the XRD, shown in Figure 1(c), con-
firms the presence of the anatase, rutile and brookite structure of TiO2 in the fiber. The XRD data of the iron
oxide and titania nanoparticle induced fiber provide evidence of considerable modification of the untreated fiber
structure (Figures 1(a)-(c)). The morphology of the fluoride treated adsorbents are shown through SEM and
TEM. SEM of the untreated fiber from grass, iron oxide, and titania nanoparticle induced fiber are shown in
Figures 2(a)-(c), respectively. The untreated micro carbon fiber exhibit carbon aggregated irregular surfaces
with a large number of macrospores and crevices of various sizes at the surface. Carbon particles look like a
T. K. Rout et al.
Figure 1. The XRD of the micro carbon from grass (a); The iron oxide based nanocomposite (b); The XRD of ti-
tania based nanocomposite (c).
Micro carbon fiber from grass (a)
20 30 40 50 60 70 80
30 40 50 60 70
Iron oxide based nanocomposite (IBNC)
Titania based nanocomposite (TBNC) (c)
T. K. Rout et al.
Figure 2. SEM images of (a) micro carbon fiber form grass, (b) IBNC, (c) TBNC.
maze of interconnecting channels, quite large at the surface and terminating in small channels in the interior .
This is indicative of carbon that is a good adsorbent base for the adsorption of pollutants from wastewaters.
Figure 2(b) showed that the particles of iron oxide grafted to carbon giving rise to a highly irregular surface
with large microspores and Figure 2(c) showed that the titania grafted carbon has irregular surfaces with various
microstructures, including rods and spheres. TEM shown in Figure 3(a) and Figure 3(b) presents agglomera-
tion of different particle sizes with spherical shapes showing both macro and micropores, and a few voids and
crevices. In contrast, the TEM of titania grafted carbon, in Figure 3(c), showed a multi-modal distribution of
particles size and solid titania rods are distributed irregularly . Figure 3(c) also clearly reveals that the outer
and inner diameter of the TiO2 rods is around 8 - 10 and 5 - 7 nm, respectively, and they have an open-end
structure. From the above studies, we observed that these metal oxides have able to convert micro carbon fiber
into nanocarbon fiber, and the same process oxides have been changed into nanoparticles of different shapes.
Scanning electron microscopy (SEM) and TEM images of the iron nanocomposite showing small nanoparticles
were distributed on the surface of the carbon fiber homogenously, decorated with nanoparticles of size 5 to 20
nm in diameter. The small size and uniformity of these nanoparticles was maintained after the 800˚C treatment;
apparently the strong interaction between the cabonfiber and the nanoparticles prevented their aggregation. This
process is very simple and scalable in both the case. The embedded metal nanoparticles on the surface of cabon
from TEM images are clearly affirming that a solid state thermal chemical reaction has been occurred between
carbon fiber and metal oxides during the process. There was no much distance between the metal nanoparticles
and the carbon surface which is indicating that the carbon has taken place in the chemical reaction. It is possible
that the carbon fiber did chemically participate in the reaction by reducing the activation energy for the trans-
formation of the metal oxides. This will require more detailed investigations in future studies. Nevertheless the
proximity of metal nanoparticle to the carbon surface is expected to alter the surface charge of the carbon fibers,
which can be probed via zeta potential study. Results of micro carbon fiber, IBNC and TBNC have been ex-
plained as under adsorption section. SEM of the fluoride treated IBNC surface is shown in Figure 3(d), which is
different from the untreated fluoride surface and has confirmed that fluorides are adsorbed on the surface re-
gardless of surface irregularities.
3.2. Effect of Contact Time and Initial Fluoride Concentration
Contact time plays a very important role in the adsorption dynamics. The effect of contact time on adsorption of
fluoride onto fiber is shown in Figure 4. Batch adsorption studies using the concentrations 2.0, 3.0, 4.0, 6.0, 8.0
and 10.0 mg/L of fluoride solution and with 0.5 g of the adsorbent were carried out at 30˚C ± 5˚C as a function
T. K. Rout et al.
Figure 3. TEM photographs of (a) micro carbon fiber, (b) IBNC, (c) TBNC,
(d) SEM image of IBNC surface after fluoride adsorption.
Figure 4. Effect of contact time on removal of fluoride on 0.5 g of adsorbents
of time to evaluate the defluoridation and adsorption rate constants. The adsorption of fluoride increases with
time and gradually attains equilibrium after 60 minutes as shown in Figure 4. Therefore 60 minutes was fixed as
minimum contact time for the maximum defluoridation of the sorbent. The adsorption of fluoride decreased
from 99.5% to 92% by increasing fluoride concentration from 2.0 to 10.0 mg/L as shown in Figure 5. Further, it
was observed that the removal curves are continuously decreasing indicating the possibility of the formation of
multilayers of fluoride ion at the pore volume and interface of the adsorbent.
3.3. Effect of pH and Adsorbent Dose
The effect of pH on removal of fluoride was examined (Figure 6). Test mixtures containing initial fluoride ion
concentration of 10 mg/L and 0.5 g/100mL of adsorbents were adjusted to various pH values both in acidic and
alkaline ranges, mixed for 60 min and analyzed for residual fluoride ion concentration by ion chromatography.
Observations from Figure 6 were made at pH levels of 2, 4, 6, 8, and 10 and these experiments were conducted
separately for all three adsorbents. The pH was maintained at the desired value within ±0.2 by adding 0.5 N
Contact time, minutes
10 20 30 60 120
IBNC Micro carbon fiber TBNC
T. K. Rout et al.
Figure 5. Effect of initial fluoride conc. on removal of fluoride on 0.5 g of
adsorbents in water.
Figure 6. Effect of pH on removal of fluoride for 0.5 g of adsorbents in water.
HNO3 or 0.1 N NaOH. The percentage of fluoride ions removed decreases with increase in pH for all three ad-
sorbents. At a pH of 2 to 4, which gives the maximum fluoride removal for both cases of metal oxide based fiber,
about 97% and 92% of fluoride ions are removed for IBNC and TBNC, respectively (Figure 6).
The effect of adsorbent dosage on the removal of fluoride ions was examined by varying the adsorbent con-
centration from 0.1 g/100mL to 0.6 g/100mLwhile all other parameters were kept constant i.e., the initial fluo-
ride ion concentration was 10 mg/L and the pH was 4. The percentage of removed fluoride ion increases with an
increase in adsorbent concentration for all three adsorbents, but after sometime, it gradually approaches a satura-
tion value, denoting an equilibrium as shown in Figure 7. IBNC removes 87% of fluoride at a dose of 0.1
g/100mLand increases to 97% removal at 0.5 g/100mL (Figure 7). The removal of fluoride ions increases from
84% to 92% when increasing the concentration of TBNC from 0.1 g/100mL to 0.5 g/100mL at a temperature of
35˚C ± 5˚C (Figure 7).
3.4. Adsorption Isotherms
The equilibrium data isotherm analysis for fluoride adsorption onto the processed fiber from grass at pH 4.0 ±
0.2 and 35˚C ± 5˚C are shown in Figure 8. Results indicate that the adsorbent has a high affinity for fluoride ion
adsorption under these conditions. As the concentration increases, adsorption capacity of fluoride also increases,
but a plateau was gradually reached for all three materials when the concentration of fluoride is beyond 7 mg/L.
The equilibrium data has been analyzed by linear regression of isotherm model equations, Freundlich and
Langmuir (Figure 9 and Figure 10, respectively). The related parameters were obtained by calculation from the
Initial fluoride concentration, mg/L
0 2 4 6 8 10 12
Micro carbon fiber
2 4 6 8 10
IBNCMicro carbon fiberTBNC
T. K. Rout et al.
Figure 7. Effect of adsorbents dosage on removal of fluoride at Ph: 4 and contact time 60
min in water.
Figure 8. Effect of concentration on fluoride removal.
Figure 9. Effect of concentration on fluoride removal fits to Freundlich model.
IBNC Micro carbon fiberTBNC
adsorbent dosage, mg/L
0.1 0.2 0.3 0.4 0.5 0.6
Equilibrium concentration of F ion in the solution (Ce), mg/L
0 1 2 3 4 5 6 7 8 9 10
IBNC Micro carbon fiberTBNC
log Ce, mg/L
−2 −1.5 −1 −0.5 0 0.5 1 1.5
IBNCMicro carbon fiberTBNC
T. K. Rout et al.
Figure 10. Effect of concentration on fluoride removal fits on Langmuir model.
values of the slopes and intercepts of the respective linear plots . The present data fit the Freundlich models
(Figure 9) well (R2
> 0.99). The average adsorption capacity (LogKF) obtained for IBNC, TBNC, and fibrous
carbon (from grass) is 0.41, 0.72, and 0.71 respectively, while the adsorption intensity (n) is found to be 2.39,
1.39, and 1.38, respectively. It is observed from the comparison of adsorption isotherms between IBNC, TBNC,
as well as fiberous carbon (from grass) that both adsorption capacity and adsorption intensity for IBNC is found
to be higher. With n > 1, there is support for the favorable adsorption of fluoride onto these biosorbents. The
linear plot for the Langmuir isotherm is shown in Figure 10. The relationship of linearity represented by Ce/qe
versus Ce shows a correlation coefficient, R2
, of 0.97 which is partially deviating from linearity. The present
data is well fit to the Freundlich isotherm inferring multilayer adsorption is taking place on the surface of the
biosorbent, due to ionic interactions. This finding is further explained by using adsorption potential theory 
which explains that adsorptive forces originating from the well-known Van der Waals interaction can attract
molecules at distances greater than a single molecular diameter. This force helps to reinforce the cohesive inter-
action between adsorbing molecules. Therefore, adsorbate molecules tend to concentrate at high energy sites on
the modified fibrous carbon surface (nano carbon fiber) and undergo precipitation. The adsorption potential is
highest in cracks and pores of the adsorbent, thus explaining the extensive adsorptive powers of fibrous carbon
with its highly developed pore structure. Figure 11 represents a heterogeneous carbon surface and the broken
lines represent the equipotential surface of having different energies (E), with the highest adsorbate concentra-
tion close to the surface, decreasing as one progresses away into the bulk of the solution. This is analogous to
the atmospheric pressure gradient in a gravitational field. At pH 4, zeta potential of the adsorbent surface for
IBNC (ξ = +4.07 mV), TBNC (ξ = −0.72 mV), and micro fibrous carbon (ξ = −5.56 mV) is found to be less
negative as shown in Figure 12. Therefore, the electrostatic interaction of fluoride ion is different depending on
the altered surface charge. IBNC has a high adsorption capacity and high adsorption intensity that may be due to
dominating electrostatic interactions as well as Van der Wall forces existing between adsorbate and adsorbent.
IBNC cultivates a highly porous structure within each granule of carbon. The wall of these pores provides in-
ternal surface area. The surface area ranges from 500 to 1500 m2
/g resulting in the extreme sorptive properties of
these materials. Although adsorption is favorable in all cases, the adsorption capacity is following the sequence
where IBNC > TBNC > micro fiberous carbon, depending on the proximity to the surface. The more cracked
and porous structure with positive surface potential has a high affinity to fluoride uptake as compared to others.
The Freundlich model, which is an indicator of surface heterogeneity of the adsorbent, explains the observed
phenomena with the experimental findings  .
The defluoridation studies of the biosorbent, i.e. processed Bermuda grass (Cynodon dactylon), have been car-
ried out in batch mode. The most excellent defluoridation occurred at the optimum time of 60 minutes allowing
for a success rate as high as 96% while keeping 10.0 mg/L fluoride concentration, 0.5 g dosage of adsorbent,
IBNC Micro carbon fiberTBNC
0 2 4 6 8 10
T. K. Rout et al.
Figure 11. Representation of adsorption potential fields in activated carbon
(Polanyi, M, 1916).
Figure 12. Effect pH on surface potential of adsorbents.
and pH 4 constant. Thus, these materials show superior adsorptive efficiency as compared to previously studied
defluoridation using natural adsorbents -. The presence of iron oxide particles is effective for the removal
of fluoride using this adsorbent. The sorption of fluoride using this adsorbent followed the Freundlich model and
the sorption process was found to be spontaneous in nature. Based on the above said description, iron oxide
nanoparticle-induced biosorbent could be used to remove fluoride selectively from water.
The authors would like to thank the Tata Steel Management for providing support for this work and permission
to publish. Special thanks to Mr. Anup Rout (Research Associate) for timely help for carrying out all experi-
ments and data generation.
 Reddy, D.R. (2009) Neurology of Endemic Skeletal Fluorosis. Neurology India, 57, 7-12.
 Jolly, S.S., Singh, I.D., Prasad, S., Sharma, R., Singh, B.M. and Mathur, O.C. (1969) An Epidemiological Study of
Endemic Fluorosis in Punjab. Indian Journal of Medical Research, 57, 1333-1346.
 Saravanan, S., Kalyani, C., Vijayarani, M., Jayakodi, P., Felix, A., Nagarajan, S., Arunmozhi, P. and Krishnan, V.
E1 E2 E3
IBNCMicro carbon fiber TBNC
0 2 4 6 8 10 12
T. K. Rout et al.
(2008) Prevalence of Dental Fluorosis among Primary Schoolchildren in Rural Areas of Chidambaram Taluk, Cud-
dalore District, Tamil Nadu. India. Indian Journal of Community Medicine, 33, 146-150.
 Shortt, H.E., Pandit, C.G. and Raghvachari, T.N.S. (1937) Endemic Fluorosis in Nellore District of South India. Indian
Medical Gazettiar, 72, 396-400.
 Susheela, A.K. (2001) Fluorosis: Indian Scienario: A Treatiseon Fluorosis. Fluorosis Research and Rural Development
Foundation, New Delhi.
 WHO (2004) Guidelines for Drinking Water Quality. World Health Organization, Geneva.
 Venkobachar, C., Iyengar, L. and Mudgal, A. (1997) Household Defluoridation of Drinking Water Using Activated
Alumina Technology. Dahi, E. and Nielsen, J.M., Eds., Proceedings of the 2nd International Workshop on Fluorosis
and Defluoridation of Water, Addis Ababa, 19-22 November 1997, International Society for Fluoride Research, Dune-
 Andezhath, S.K. and Ghosh, G. (2000) Fluorosis Management in India: The Impact Due to Networking between
Health and Rural Drinking Water Supply Agencies. IAHS AISH Publication, 260, 159-165.
 USEPA 440/1-74-024-a (1974) Development Document for Effluent Limitations Guidelines and New Source Per-
formance Standards for the Steel Making Segment of the Iron and Steel Manufacturing Point Source Category.
 USEPA 440/1-75/040 (1975) Development Document for Interim Final Effluent Limitation Guidelines and Proposed
New Source Performance Standards for the Common and Precious Metals Segment of the Electroplating Point Source
 USEPA 440/1-75/034-a, Group l, Phasell (1975) Development Document for Effluent Limitations Guidelines and New
Source Performance Standards for the Pressed and Blown Glass Segment of the Glass Manufacturing Point Source
Category. Washington DC.
 UNICEF’s Position on Water Fluoridation (2005) Fluoride in Water: An Overview.
 Agarwal, V., Vaish, A.K. and Vaish, P. (1997) Groundwater Quality: Focus on Fluoride and Fluorosis in Rajasthan.
Current Science, 73, 743-746.
 Passmore, R., Nicol, B.M., Rao, M.N., Beaton, G.H. and Demayer, E.M. (1974) Handbook on Human Nutritional Re-
quirements. World Health Organization Monograph Series, No. 61, Geneva, 1-66.
 Teotia, S.P. and Teotia, M. (1984) Endemic Fluorosis in India: A Challenging National Health Problem. Journal of the
Association of Physicians of India, 32, 347-352.
 Rajiv Gandhi National Drinking Water Mission (1993) Prevention and Control of Fluorosis in India. Ministry of Rural
Development, New Delhi.
 Kotecha, P.V., Patel, S.V., Bhalani, K.D., Shah, D., Shah, V.S. and Mehta, K.G. (2012) Prevalence of Dental Fluorosis
& Dental Caries in Association with High Levels of Drinking Water Fluoride Content in a District of Gujarat, India.
Development Foundation, New Delhi. Indian Journal of Medical Research, 135, 873-877.
 Yadav, S., Khan, T.I., Gupta, S., Gupta, A.B. and Yadava, R.N. (1999) Fluorosis in India with Special Reference to
Rajasthan. In: Proceedings of the International Conference on Water, Environment, Ecology, Socioeconomics and
Health Engineering (WEESHE), Seoul National University, Seoul, 3-10.
 Monroy, S.D. (2011) Fluoride Properties, Applications and Environmental Management, 111-136.
 Chauhan, D., Chauhan, T., Sachdev, V. and Kirtaniya, B.C. (2012) A Study of Prevalence and Severity of Dental
Fluorosis among School Children in a Northern Hilly State of India. SRM Journal of Research in Dental Sciences, 3,
 Grimaldo, M., Turrubiartes, F., Milan, J., Pozos, A., Alfaro, C. and Diaz-Barriga, F. (1997) Endemic Fluorosis in San
Luis Potosi, Mexico. Fluoride, 30, 33-40.
 Brudevold, F. and Soremark, R. (1967) Structural and Chemical Organization of Teeth, Vol. 2. Miles, A.G.W., Ed.,
Academic Press, New York and London, 247.
 Bansiwal, A., Pillewan, P., Biniwale, R.B. and Rayalu, S.S. (2010) Copper Oxide Incorporated Mesoporous Alumina
for Defluoridation of Drinking Water. Microporous and Mesoporous Materials, 129, 54-61.
 Bhaumika, M., Leswifia, T.Y., Maity, A., Srinivasu, V.V. and Onyango, M.S. (2011) Removal of Fluoride from
Aqueous Solution by Polypyrrole/Fe3O4 Magnetic Nanocomposite. Journal of Hazardous Materials, 186, 150-159.
 Bia, G., Pauli, C.P.D. and Borgnino, L. (2012) The Role of Fe(III) Modified Montmorillonite on Fluoride Mobility:
T. K. Rout et al.
Adsorption Experiments and Competition with Phosphate. Journal of Environmental Management, 100, 1-9.
 Chen, N., Zhang, Z., Feng, C., Li, M., Zhu, D. and Sugiura, N. (2011) Studies on Fluoride Adsorption of Iron-Im-
pregnated Granular Ceramics from Aqueous Solution. Materials Chemistry and Physics, 125, 293-298.
 Das, N., Pattanaik, P. and Das, R. (2005) Defluoridation of Drinking Water Using Activated Titanium Rich Bauxite.
Journal of Colloid and Interface Science, 292, 1-10. http://dx.doi.org/10.1016/j.jcis.2005.06.045
 Li, Y.H., Wang, S., Cao, A., Zhao, D., Zhang, X., Xu, C., Luan, Z., Ruan, D., Liang, J., Wu, D. and Wei, B. (2001)
Adsorption of Fluoride from Water by Amorphous Alumina Supported on Carbon Nanotubes. Chemical Physics Let-
ters, 350, 412-416. http://dx.doi.org/10.1016/S0009-2614(01)01351-3
 Yan, X.R., Song, K.X., Wang, J.P., Hu, L.C. and Yang, Z.H. (1998) Preparation of CeO2-TiO2/SiO2 and Its Removal
Properties for Fluoride Ions. Journal of Rare Earths, 16, 279-280.
 Cui, H., Qian, Y., An, H., Sun, C., Zhai, J. and Li, Q. (2012) Electrochemical Removal of Fluoride from Water by
PAOA Modified Carbon Felt Electrodes in a Continuous Flow Reactor. Water Research, 46, 3943-3950.
 Puri, B.K. and Balani, S. (2000) Trace Determination of Fluoride Using Lanthanum Hydroxide Supported on Alumina.
Journal of Environmental Science and Health, Part A, 35, 109-121. http://dx.doi.org/10.1080/10934520009376957
 Ansari, M., Kazemipour, M., Dehghani, M. and Kazemipour, M. (2011) The Defluoridation of Drinking Water Using
Multi-Walled Carbon Nanotubes. Journal of Fluorine Chemistry, 132, 516-520.
 Swain, S.K., Patnaik, T., Singh, V.K., Jha, U., Patel, R.K. and Dey, R.K. (2011) Kinetics, Equilibrium and Thermody-
namic Aspects of Removal of Fluoride from Drinking Water Using Meso-Structured Zirconium Phosphate. Chemical
Engineering Journal, 171, 1218-1226. http://dx.doi.org/10.1016/j.cej.2011.05.030
 Cherry, J.M. (1970) Fluoride Recovery in Phosphate Manufacture. Water and Waste Engineering, 7, D5.
 Mohapatra, M., Hariprasad, D., Mohapatra, L., Anand, S. and Mishra, B.K. (2012) Mg-Doped Nano Ferrihydrite—A
New Adsorbent for Fluoride Removal from Aqueous Solutions. Applied Surface Science, 258, 4228-4236.
 Guo, Q. and Reardon, E.J. (2012) Fluoride Removal from Water by Meixnerite and Its Calcination Product. Applied
Clay Science, 56, 7-15. http://dx.doi.org/10.1016/j.clay.2011.11.013
 Ma, W., Ya, F., Wang, R. and Zhao, Y.Q. (2008) Fluoride Removal from Drinking Water by Adsorption Using Bone
Char as a Biosorbent. International Journal of Environmental Technology and Management, 9, 59-69.
 Dey, S., Swarup, D., Saxena, A. and Dan, A. (2011) In Vivo Efficacy of Tamarind (Tamarinds indica) Fruit Extract on
Experimental Fluoride Exposure in Rats. Research in Veterinary Science, 91, 422-425.
 Mandal, S. and Mayadevi, S. (2009) Defluoridation of Water Using as-Synthesized Zn/Al/Cl Anionic Clay Adsorbent:
Equilibrium and Regeneration Studies. Journal of Hazardous Materials, 167, 873-878.
 Kumar, N.P., Kumar, N.S. and Krishnaiah, A. (2011) Defluoridation of Water Using Tamarind (Tamarindus indica)
Fruit Cover: Kinetics and Equilibrium Studies. Journal of the Chilean Chemical Society, 57, 1224-1231.
 Mohan, X.D.D., Pittman Jr., C.U. and Yang, S. (2012) Remediating Fluoride from Water Using Hydrous Zirconium
Oxide. Chemical Engineering Journal, 198-199, 236-245. http://dx.doi.org/10.1016/j.cej.2012.05.084
 Poursaberi, T., Hassanisadi, M., Torkestani, K. and Zare, M. (2012) Development of Zirconium (IV)-Metalloporphyrin
Grafted Fe3O4 Nanoparticles for Efficient Fluoride Removal. Chemical Engineering Journal, 189-190, 117-125.
 Ramanjaneyulu, V., Jaipal, M., Yasovardhan, N. and Sharada, S. (2013) Kinetic Studies on Removal of Fluoride from
Drinking Water by Using Tamarind Shell and Pipal Leaf Powder. International Journal of Emerging Trends in Engi-
neering and Development, 5, 146.
 Tripathy, S.S., Bersillon, J.L. and Gopal, K. (2006) Removal of Fluoride from Drinking Water by Adsorption onto
Alum-Impregnated Activated Alumina. Separation and Purification Technology, 50, 310-317.
 Langmuir, I. (1916) The Constitution and Fundamental Properties of Solids and Liquids. Part I. Solids. Journal of the
American Chemical Society, 38, 2221-2295. http://dx.doi.org/10.1021/ja02268a002
 Sivasamy, A., Singh, K.P., Mohan, D. and Maruthamuthu, M. (2001) Studies on Defluoridation of Water by Coal-
Based Sorbents. Journal of Chemical Technology and Biotechnology, 76, 717-722.
T. K. Rout et al.
 Sivasankar, V., Murugesh, S., Rajkumar, S. and Darchen, A. (2013) Cerium Dispersed in Carbon (CeDC) and Its Ad-
sorption Behavior: A First Example of Tailored Adsorbent for Fluoride Removal from Drinking Water. Chemical En-
gineering Journal, 214, 45-54. http://dx.doi.org/10.1016/j.cej.2012.10.023
 Subramanian, E. and Ramalakshmi, R.D. (2010) Pristine, Purified and Polyaniline-Coated Tamarind Seed (Tamarindus
indica) Biomaterial Powders for Defluoridation: Synergism and Enhancement in Fluoride Adsorption by Polyaniline
Coating. Journal of Scientific and Industrial Research, 69, 621-628.
 Turner, B.D., Binning, P. and Stipp, S.L.S. (2005) Fluoride Removal by Calcite: Evidence for Fluorite Precipitation
and Surface Adsorption. Environmental Science & Technology, 39, 9561-9568. http://dx.doi.org/10.1021/es0505090
 Wajima, T., Umeta, Y., Narita, S. and Sugawara, K. (2009) Adsorption Behavior of Fluoride Ions Using a Titanium
Hydroxide-Derived Adsorbent. Desalination, 249, 323-330. http://dx.doi.org/10.1016/j.desal.2009.06.038
 Camacho, L.M., Torres, A., Saha, D. and Deng, S. (2010) Adsorption Equilibrium and Kinetics of Fluoride on Sol-Gel-
Derived Activated Alumina Adsorbents. Journal of Colloid and Interface Science, 349, 307-313.
 Vithanagea, M., Jayarathnaa, L., Rajapakshaa, A.U., Dissanayakea, C.B., Bootharajub, M.S. and Pradeep, T. (2012)
Modeling Sorption of Fluoride on to Iron Rich Laterite. Colloids and Surfaces A: Physicochemical and Engineering
Aspects, 398, 69-75. http://dx.doi.org/10.1016/j.colsurfa.2012.02.011
 Sakhare, N., Lunge, S., Rayalu, R., Bakardjiva, S., Subrt, J., Devotta, S. and Labhsetwar, N. (2012) Defluoridation of
Water Using Calcium Aluminate Material. Chemical Engineering Journal, 203, 406-414.
 Chakrabarty, S. and Sarma, H.P. (2012) Defluoridation of Contaminated Drinking Water Using Neem Charcoal Ad-
sorbent: Kinetics and Equilibrium Studies. International Journal of ChemTech Research, 4, 511-516.
 Sylvester, R.O., Oglesby, R.T., Carlson, D.A. and Christman, R.F. (1967) Factors Involved in the Location and Opera-
tion of an Aluminium Reduction Plant. Proceedings of the 22nd Industrial Waste Conference, Purdue, 2-4 May 1967,
 Romanos, J., Beckner, M., Rash, T., Firlej, L., Kuchta, B., Yu, P., et al. (2012) Nanospace Engineering of KOH Acti-
vated Carbon. Nanotechnology, 23, Article ID: 015401. http://dx.doi.org/10.1088/0957-4484/23/1/015401
 Wang, S.G., Li, Y.H., Zhao, D., Xu, C.L., Luan, Z.K., Liang, J. and Wu, D.H. (2002) Preparation of Alumina Sup-
ported on Carbon Nanotubes and Its Application in Fluoride Adsorption from an Aqueous Solution. Chinese Science
Bulletin, 47, 722-724. http://dx.doi.org/10.1360/02tb9162
 Sarkar, M., Banerjee, A. and Pramanick, P.P. (2006) Kinetics and Mechanism of Fluoride Removal Using Laterite. In-
dustrial & Engineering Chemistry Research, 45, 5920-5927.
 Sivasankar, V., Rajkumar, S., Murugesh, S. and Darchen, A. (2012) Influence of Shaking or Stirring Dynamic Methods
in the Defluoridation Behaviour of Activated Tamarind Fruit Shell Carbon. Chemical Engineering Journal, 197, 162-
 Maliyekkal, S.M., Sharma, A.K. and Philip, L. (2006) Manganese-Oxide-Coated Alumina: A Promising Sorbent for
Defluoridation of Water. Water Research, 40, 3497-3506. http://dx.doi.org/10.1016/j.watres.2006.08.007
 Gupta, A.K., Deva, D., Sharma, A. and Verma, N. (2009) Adsorptive Removal of Fluoride by Micro-Nanohierarchal
Web of Activated Carbon Fibers. Industrial & Engineering Chemistry Research, 48, 9697-9707.
 Sundaram, C.S., Viswanathan, N. and Meenakshi, S. (2009) Defluoridation of Water Using Magnesia/Chitosan Com-
posite. Journal of Hazardous Materials, 163, 618-624. http://dx.doi.org/10.1016/j.jhazmat.2008.07.009
 Kishore, M. and Hanumantharao, Y. (2010) Validation of Defluoridation Method with “Acacia Arabica” Plant by
Product through 2n
Factorial Experimentation—A Statistical Approach. International Journal of Applied Biology and
Pharmaceutical Technology, 1, 1230-1235.
 Martin, R.J. and Ng, W.J. (1997) The Repeated Exhaustion and Chemical Regeneration of Activated Carbon. Water
Research, 21, 961-965. http://dx.doi.org/10.1016/S0043-1354(87)80014-3
 Mondal, N.K., Bhaumik, R., Baur, T., Das, B., Roy, P. and Datta, J.K. (2012) Studies on Defluoridation of Water by
Tea Ash: An Unconventional Biosorbent. Department of Environmental Science, The University of Burdwan, Burd-
wan, Chemical Science Transactions, 1, 239-256.
 American Public Health Association (2007) Standard Methods for the Examination of Water and Waste Water. 14th
 Ayoob, S. and Gupta, A.K. (2008) Insights into Isotherm Making in the Sorptive Removal of Fluoride from Drinking
Water. Journal of Hazardous Materials, 152, 976-985. http://dx.doi.org/10.1016/j.jhazmat.2007.07.072
T. K. Rout et al.
 Sekino, T. (2010) Synthesis and Applications of Titanium Oxide Nanotubes. In: Kijima, T., Ed., Inorganic and Metal-
lic Nan Tubular Materials, Recent Technologies and Applications, X, Springer-Verlag, Berlin Heidelberg, 17-32.
 Biswas, K., Bandhoyapadhyay, D. and Ghosh, U.C. (2007) Adsorption Kinetics of Fluoride on Iron(III)-Zirconium(IV)
Hybrid Oxide. Adsorption, 13, 83-94. http://dx.doi.org/10.1007/s10450-007-9000-1
 Polanyi, M. (1916) Adsorption of Gases by Asolid Non-Volatile Adsorbent. Verhandlungen der Physikalischen Ge-
sellschaftzu Berlin, 18, 55.
 Perrich, J.R. (1981) Activated Carbon Adsorption for Waste Water Treatment. CRC Press, Inc., Boca Raton.
 Giles, C.H., MacEwan, T.H., Nakhwa, S.N. and Smith, D. (1960) Studies in Adsorption. Part XI. A System of Classi-
fication of Solution Adsorption Isotherms, and Its Use in Diagnosis of Adsorption Mechanisms and in Measurement of
Specific Surface Areas of Solids. Department of Chemical Technology, The Royal College of Science & Technology,